defects and grading after kiln drying hardwood lumber sawn ... drying treatments (one kiln charge...
Post on 01-Jun-2020
Embed Size (px)
PEER-REVIEWED ARTICLE bioresources.com
Wiedenbeck et al. (2019). “Dry kiln schedules,” BioResources 14(2), 4085-4099. 4085
Defects and Grading after Kiln Drying Hardwood Lumber Sawn from Small-diameter Logs
Jan K. Wiedenbeck,a,* Matthew S. Scholl,b Paul R. Blankenhorn,c and Chuck D. Ray d
Close inspection of black cherry (Prunus serotina), sugar maple (Acer saccharum), and northern red oak (Quercus rubra) lumber, before and after kiln drying, revealed the factors that can affect the quality of kiln-dried lumber from small-diameter logs. Species-specific kiln drying schedules, with temperature and humidity modifications formulated by a kiln drying expert, were employed in this study to determine whether alternate drying protocols could improve the drying outcomes. Comparing lumber grades of individual boards before and after drying indicated that overall grade loss in the kiln was common but was affected by both species and the applied drying schedule. Most lumber defects were attributed to stresses that occurred during the drying process and were more prevalent in the post-drying inspection, with bow defects being the exception. The modified kiln schedules improved the drying defect outcomes for the black cherry and red oak compared with the conventional schedules for these species. For the sugar maple, the schedule-based improvement was less consistent. For the black cherry and red oak, the percentage of boards whose grade decreased using conventional kiln protocols was approximately 10% lower than that of the lumber that was dried using the modified kiln protocols. Sugar maple had a smaller change of 7%.
Keywords: Small-diameter hardwoods; Lumber recovery; Lumber grade; Dry kiln schedule;
Contact information: a: USDA Forest Service, Northern Research Station, 301 Hardwood Lane, Princeton,
WV 24740 USA; b: Great Southern Wood Preserving, 2290 Plunkett Road NW, Conyers, GA 30012 USA;
c: Department of Ecosystem Science and Management (retired), Forest Resources Bldg., University Park,
PA 16802 USA; d: Department of Ecosystem Science and Management (retired), Forest Resources Bldg.,
University Park, PA 16802 USA; *Corresponding author: email@example.com
Lumber used for high-value appearance grade products must be dried to a moisture
content that suits the interior environment where the final product will be used; in North
America this usually means it must be kiln-dried to a moisture content of 8% to 10%. The
stresses that arise during the drying process frequently lead to defects in the lumber that
reduce its grade, value, and utility. When assessing the potential for using smaller diameter
hardwood logs for the manufacturing of hardwood lumber, the quality and value of the
kiln-dried lumber is the ultimate deciding factor.
A few studies on the lumber recovery potential of small-diameter hardwood logs
(generally defined as logs with a diameter less than 11 at the small end) have evaluated the
lumber volume and grade yields for “green” lumber (before drying) (Emanuel 1983;
Hamner et al. 2006; Perkins et al. 2008). Green lumber recovery rates may be of interest
to lower and mid-value lumber markets, such as pallet, container, and fencing
manufacturers; however, the current green recovery information is not sufficient for lumber
buyers who manufacture appearance-grade products that require kiln-dried lumber.
PEER-REVIEWED ARTICLE bioresources.com
Wiedenbeck et al. (2019). “Dry kiln schedules,” BioResources 14(2), 4085-4099. 4086
Scholl et al. (2008) studied the lumber grade yields and other quality characteristics
of black cherry (Prunus serotina) lumber sawn from small-diameter logs and dried in a
kiln. Scholl et al. (2008) identified the defects and grade/value losses that arose during the
kiln drying process with both a conventional black cherry kiln schedule and two alternate
schedules. Scholl (2006) evaluated the recoveries from small-diameter red oak (Quercus
rubra), sugar maple (Acer saccharum), and black cherry logs, and many utilization
characteristics were measured before and after the kiln drying process. Wiedenbeck et al.
(2017) highlighted the overall lumber volume and value recovery results obtained by
Scholl (2006) for all three species with both the green and kiln-dried moisture content
conditions. After kiln drying, the distribution of the lumber grades was lower for all three
species when compared with the lumber grades before it was dried (approximately 25% of
the boards dropped to a lower grade value) (Wiedenbeck et al. 2017). Eucalyptus globulus
harvested from 10-year-old plantations yielded a high proportion of low-grade sawn
boards, but changes in grade after kiln drying were not examined (Yang et al. 2002).
Changes in warpage amounts were compared before and after drying with bow-type
distortions reduced in the kiln drying process while crook (spring)-type distortion results
varied (Yang et al. 2002).
The principal goal of the research by Scholl (2006) was to develop information on
the quality and value of the lumber produced from small-diameter hardwood logs of three
important commercial species in the U.S. and many global markets, namely red oak, hard
maple, and black cherry. Not only did that research produce original insights into basic
lumber recovery from small-diameter logs after kiln drying (Wiedenbeck et al. 2017), it
also explored the effects of different dry kiln temperatures and relative humidity schedules
on the quality and value outcomes for each species.
The objective of this research was to discover whether newly devised, alternate dry
kiln schedules for drying lumber recovered from small-diameter hardwood logs result in
similar or different levels of drying caused defects as compared to results obtained when
conventional dry kiln schedules are used in drying black cherry, sugar maple, and red oak.
Log Samples The log samples were obtained from small-diameter trees harvested in northern and
central Pennsylvania. The tree selection was neither random nor deliberate. Logs were
provided by cooperating sawmills and were delivered to the collection/processing site over
a period of several weeks. All of the stems delivered to the study team were included in the
sample. The stems had various lengths when received. They were then bucked into lengths
of 8 ft 4 in, numbered for tracking purposes, and end-sealed. One or two 8-ft logs were
obtained from each stem. The overall sample consisted of 159 logs from 130 black cherry
trees, 132 logs from 113 sugar maple trees, and 87 logs from 70 red oak trees. The small-
end diameters inside of the bark (scaling diameter) of the study logs were less than or equal
to 12 in. The proportion of logs with diameters of less than 10 in was the highest for the
black cherry (63%) and lower for the sugar maple and red oak (31% and 40%,
PEER-REVIEWED ARTICLE bioresources.com
Wiedenbeck et al. (2019). “Dry kiln schedules,” BioResources 14(2), 4085-4099. 4087
Log Breakdown and Kiln Drying The logs were sawn on a portable sawmill (Timber Harvester, Waterloo, NY) at
Penn State University (University Park, USA) by a single experienced sawmill operator.
The opening face of each log (i.e., the placement of the first sawline) was the log face
opposite from the highest quality face on the log. Each sawn board was numbered so that
it could be tracked throughout the study. Within 24 h of being sawn, each board was
evaluated for the full set of stress-induced defects, which are often exacerbated by the
lumber drying process. These defects include end checks, surface checks, shakes, bows,
twists, crooks, and cups. The boards were also graded using the grade rules of the National
Hardwood Lumber Association (NHLA 2014).
The lumber was hand stacked into packs that were 8 ft (length) × 4 ft (width) × 4.5
ft (height). The kiln used was a steam-heated kiln (Custom Built in 1965, with Irvington-
Moore and Allen-Bradley monitoring and control systems) with a capacity of 1500 board
feet (BF). A conventional and two experimental kiln schedules were used in this project.
When the logs were sawn into lumber, it was apparent that the red oak sample had a
bacterial infection, which is not uncommon. Bacterially infected red oak must be dried
more carefully to prevent deep surface checks, honeycomb, and ring failure. A dry kiln
schedule for BI red oak was used according to the Dry Kiln Operator’s Manual (Simpson
2001) and was incorporated into this study as the conventional schedule for the red oak.
The first modified kiln (MOD-1) schedule used for each species lowered the final
dry- and wet-bulb setting, while the second modified (MOD-2) schedule decreased both
the initial and final dry- and wet-bulb settings. It was hypothesized that the lower final dry-
and wet-bulb temperatures slowed the rate of warping in the lumber during the final stages
of drying because of the premature release of drying stresses. It was proposed that lumber
dried using the lower ini